Dunford, Alan (2013) Friction and the texture of
aggregate particles used in the road surface course.
PhD thesis, University of Nottingham.
Access from the University of Nottingham repository:
Copyright and reuse:
The Nottingham ePrints service makes this work by researchers of the University of
Nottingham available open access under the following conditions.
Copyright and all moral rights to the version of the paper presented here belong to
the individual author(s) and/or other copyright owners.
To the extent reasonable and practicable the material made available in Nottingham
ePrints has been checked for eligibility before being made available.
Copies of full items can be used for personal research or study, educational, or
not-for-profit purposes without prior permission or charge provided that the authors, title
and full bibliographic details are credited, a hyperlink and/or URL is given for the
original metadata page and the content is not changed in any way.
Quotations or similar reproductions must be sufficiently acknowledged.
Please see our full end user licence at:
A note on versions:
The version presented here may differ from the published version or from the version of
record. If you wish to cite this item you are advised to consult the publisher’s version. Please
see the repository url above for details on accessing the published version and note that
access may require a subscription.
AGGREGATE PARTICLES USED IN THE
ROAD SURFACE COURSE
Thesis submitted to the University of Nottingham for the degree of Doctor of Philosophy
Skid resistance, the road surface’s contribution to friction, is a crucial property of a road surface course required to maintain a safe and serviceable road network.
Measurement of skid resistance is restricted by the need to measure the forces acting on a rubber wheel or slider while it is dragged across the surface. If the skid resistance of the road could be determined without the need for contact then measurement could be cheaper and more thorough. One route to achieving this goal is by measurement of the texture of the road that generates the friction experienced by a sliding tyre. However, the form and scale of the texture required is not well defined.
The work presented in this thesis attempts to establish a robust methodology for measurement of texture on the surfaces of aggregate particles (the main constituent of the road surface course) so that it can be compared with friction. The stages of development are described in detail and the methodology is employed to examine the changing texture on two types of aggregate.
The mechanisms by which these aggregates polish, methods for characterising their surface texture, and the consequences for the friction they are able to generate are explored.
Where experiments described in this thesis have been published elsewhere, references are given in the text. In addition, elements of the work presented in Chapters 5, 6 and 7 of this thesis have been published as follows.
Dunford, A. (2010). PPR538. Measuring skid resistance without contact;
2009-2010 progress report. Crowthorne: TRL.
Dunford, A. M., Parry, A. R., Shipway, P. H., & Viner, H. E. (2012). Three-dimensional characterisation of surface texture for road stones undergoing simulated traffic wear. Wear 292, 188-196.
There are a great many people to acknowledge and I have run out of words to thank them all properly so they appear here as a list of names.
Dunfords: Catherine, Raspberry, Diana, Bryan, Daniel, Mary Supervisors: Tony Parry, Helen Viner, Phil Shipway
TRL and (in alphabetical order) Emma Benbow, Stuart Brittain, Nathan Dhillon, Kevin Green, Martin Greene, Rod Kimber, Richard Lodge, Stuart McRobbie, Derek Meachen, Neil Paulley, Peter Roe, Peter Sanders, Richard Woodward, Alex Wright, Dean Wright
NPL and Richard Leach, Claudiu Giusca, James Claverley UoN and Nigel Neate, Nick Thom
Highways Agency and Louise Caudwell, Ramesh Sinhal Lafarge and Paul Edwards, John Harris, Robert Gossling David Woodward and Richard Ellis of University of Ulster
1 Introduction 1
1.1 Background 2
1.2 Research aims 5
1.3 Description of following chapters 6
1.4 References 8 2 Literature review 9 2.1 Friction theory 11 2.1.1 Classical friction 11 2.1.2 Rubber friction 12 2.1.3 Lubrication 20 2.1.4 Summary 22
2.2 Road surface texture 24
2.3 Measuring texture 30
2.3.1 Standard methods for measuring road surface texture 30
2.3.2 Less common or future field measurement techniques 31
2.3.3 Laboratory techniques for measurement of surface texture 35
2.4 Texture characterisation 39
2.4.1 Standard characterisation of road surface texture 39
2.4.2 Experimental characterisation of road surface texture 41
2.4.3 Laboratory 49
2.5 Factors affecting skid resistance 57
2.5.1 Surface texture 57
2.5.2 Other factors affecting skid resistance 63
2.6 Aggregates 67
2.6.1 Specification of road stones 67
2.6.2 Geology of typical road stones 71
2.7 Summary 75
2.8 References 78
3 Feasibility studies 85
3.1 Collecting information about road surface texture 86
3.2 Using information contained in high resolution images of
aggregate surfaces 91
3.3 Developing a methodology for measuring and characterising
aggregate surface texture 98
3.3.1 Texture measurements 98
3.3.3 Comparing texture and friction 104
3.4 Discussion 107
3.5 References 109
4 First attempts at an improved methodology for
examination of surface texture changes 111
4.1 Methodology 112
4.1.1 Specimen 112
4.1.2 Polishing 114
4.1.3 Photography 115
4.1.4 Surface replication 115
4.1.5 Scanning electron microscopy 116
4.1.6 Surface texture measurement 117
4.2 Photography 118
4.3 Scanning electron microscopy 123
4.4 Surface texture measurements 128
4.4.1 Analysis using raw data and Microsoft Excel 128
4.4.2 Texture analysis using data visualisation software 129
4.4.3 Texture analysis using bespoke software 134
4.5 Discussion 137
4.6 References 139
5 Development of a robust methodology to examine
surface texture changes 141
5.1 Polishing in the laboratory 142
5.1.1 Methodology for comparing W-S polishing with traffic
5.1.2 Progressive polishing of aggregate specimens 147
5.2 Measuring friction in the laboratory 149
5.2.1 Friction measurement using the Wehner-Schulze machine 149
5.2.2 Details of the W-S friction measurement system 150
5.2.3 Measurements of friction for comparison with surface
5.3 Texture measurement areas and alignment 155
5.4 Texture measurement 161
5.5 Paint erosion 164
5.6 Aggregates 166
5.7 References 168
6.3 Changes that become apparent when considering smaller
areas of surface 179
6.4 Analysis in two dimensions 184
6.5 Discussion 187
7 Quantitative analysis of changes in texture during polishing 189
7.1 Development of model profiles against which to examine the
surface characterisation techniques 191
7.2 Manual analysis 194
7.3 Power Spectral Density 199
7.4 Fractal analysis 207
7.5 Introduction to roughness parameters 212
7.6 Height parameters 216
7.7 Peak height and peak density 226
7.8 Peak gradient 233
7.9 Volumetric parameters 235
7.10 Height distribution 239
7.11 Correlation between roughness parameters and friction 244
7.12 Inclusion of results from dolerite surfaces 248
7.13 Discussion 250
7.14 References 252
8 Summary and discussion 255
8.1 Introduction 256
8.2 Literature review 257
8.3 Feasibility studies 258
8.4 First attempts at an improved methodology 259
8.5 Development of a robust methodology 260
8.6 Qualitative analysis of changes in texture 261
8.7 Quantitative analysis of changes in texture 262
8.8 General discussion 264
8.9 References 265
9 Conclusions and recommendations for further work 267
9.1 Conclusions 268
9.2 Recommendations for further work 271
This chapter introduces the work described in this thesis. A background to the project is given by way of justification for the work before broad research questions and specific research aims are presented.
The number of road accidents and casualties reported in the UK has not changed as much, in the last sixty years, as the length of our roads and the number of vehicles using them; Figure 1.1 shows the relatively small fluctuations in thousands of casualties and the substantial increase in billions of vehicle miles. Accident statistics are therefore often presented in terms of a casualty rate per billion vehicle miles (Figure 1.2), which demonstrates a significant reduction so that, despite the increase in road traffic, travel seems to be getting safer (Department for Transport, 2011). The general improvement is often attributed to government safety campaigns (seatbelt and drink-drive campaigns for example) and improved vehicle safety features such as anti-lock braking. Although often un-credited, developments in road surfacing, condition monitoring and policies have played an important part in reducing skidding accidents. In particular, it has been shown that skid resistance is linked to accident risk. For example, Rogers and Gargett (1991) demonstrated an increase in risk for road sites with lower skid resistance and Viner et al (2005) analysed skid resistance and accident data and made conclusions including “For dual carriageways there is a statistically significant trend for accident risk to increase at locations with lower skid resistance”.
0 50 100 150 200 250 300 350 400 450 1 9 5 0 1 9 5 2 1 9 5 4 1 9 5 6 1 9 5 8 1 9 6 0 1 9 6 2 1 9 6 4 1 9 6 6 1 9 6 8 1 9 7 0 1 9 7 2 1 9 7 4 1 9 7 6 1 9 7 8 1 9 8 0 1 9 8 2 1 9 8 4 1 9 8 6 1 9 8 8 1 9 9 0 1 9 9 2 1 9 9 4 1 9 9 6 1 9 9 8 2 0 0 0 2 0 0 2 2 0 0 4 2 0 0 6 2 0 0 8 2 0 1 0 N u m b e r o f c a s u a lt ie s ( th o u s a n d s ) o r n u m b e r o f v e h ic le m il e s ( b il li o n s ) Year
All reported casualties Traffic, all vehicles
Figure 1.2 UK casualty rate
In England, the Highways Agency has responsibility for providing a safe and serviceable trunk road network (i.e. motorways and most major roads) and one crucial element of this is to ensure that the roads have adequate skid resistance. For more than two decades, the Agency’s “skid policy” has been to monitor the skid resistance of the network by carrying out thorough routine measurements (Design Manual for Roads and Bridges, 2004). The same, or a similar, policy has typically been adopted by those authorities with responsibility for all other parts of the UK road network. Investigation of better ways to make measurements of skid resistance is where the work described in this thesis began.
Skid resistance can be measured by various types of equipment, but all devices suitable for routine use rely on measuring the forces generated when a rubber tyre or slider is dragged across a wetted surface. The logistics of measuring using specialist devices means that surveys are costly and time consuming. There are other major disadvantages to making measurements in this way:
For logistical and legal reasons measurements are confined to a small proportion of the road width, generally a single, continuous line in the nearside wheel path of lane 1. Although this is generally supposed to be the area of lowest skid resistance it is possible that other areas of low skid resistance may go undetected.
0 500 1,000 1,500 2,000 2,500 3,000 3,500 4,000 4,500 5,000 1 9 5 0 1 9 5 2 1 9 5 4 1 9 5 6 1 9 5 8 1 9 6 0 1 9 6 2 1 9 6 4 1 9 6 6 1 9 6 8 1 9 7 0 1 9 7 2 1 9 7 4 1 9 7 6 1 9 7 8 1 9 8 0 1 9 8 2 1 9 8 4 1 9 8 6 1 9 8 8 1 9 9 0 1 9 9 2 1 9 9 4 1 9 9 6 1 9 9 8 2 0 0 0 2 0 0 2 2 0 0 4 2 0 0 6 2 0 0 8 2 0 1 0 N u m b e r o f c a s u a lt ie s p e r b il li o n v e h ic le m il e s Year Casualty rate
Skid resistance measurements made through physical contact vary with the speed of measurement (the friction/speed relationship is described in more detail in Section 2.5). Measurement errors can be introduced when measurement vehicles are unable to maintain a constant speed amongst live traffic, typically for safety reasons. If skid resistance could be measured, or at least estimated, without contact, then these limitations could be avoided, potentially improving safety. A better, or more complete, understanding of the condition of the road network could lead to improved targeting of maintenance which, in turn, could lead to increased sustainability and cost benefit.
It is thought that the skid resistance of a road is affected by its surface texture, and in particular, by texture with wavelengths less 10 mm. It is already possible to measure texture without contact for wavelengths of 2 mm and higher, but these features are thought, and have been shown empirically, to determine the rate of change in skid resistance with speed (as mentioned above). The actual level of skid resistance is supposedly related to texture on a somewhat finer scale and, unfortunately, this conjecture is almost as far as the theory goes. To complicate matters further, a road’s skid resistance is not a constant property, not least because the surface’s component parts (mainly the coarse aggregate used in construction) respond to the polishing action of traffic in conjunction with the prevailing weather conditions.
The subject of this thesis is the investigation of aggregate particle (road stone) surface texture, with particular reference to the influence of this texture on the skid resistance of the road pavement and the way it changes as it is polished, either by traffic or in the laboratory. As the work progressed it became clear that there was a need to first develop a robust methodology and so the experimental work described in later chapters is of a practical nature.
Setting aside the technical difficulty with measuring detailed texture of sufficiently small wavelengths at sufficiently high speeds, there are a number of distinct questions to answer before contactless measurement of skid resistance is possible:
Which wavelengths of texture are important? There may be limits above or below which the texture is less important, or a continuum may be required.
What form does the texture take? This may be different for the numerous different types of materials used to make road surfaces. How can the relevant texture be numerically characterised?
What is the link between texture and skid resistance?
Devising a robust methodology for proper investigation is a crucial step which has to be undertaken first. The aims of the research presented in the following chapters can be summarised as follows:
Develop a methodology that will allow observation of changes in surface texture on aggregate particle surfaces as they are polished in the laboratory
Observe changes in texture on more than one type of aggregate and compare the forms of the texture present and the mechanisms by which texture changes
Evaluate several numerical methods for their ability to characterise the texture found on aggregate particle surfaces.
Description of following chapters
This thesis is split into nine chapters. Their titles and contents are as follows:
The current chapter introduces the topic of study and states the general questions and specific aims of the research presented in subsequent chapters.
2. Literature review
Discusses theories proposed for friction generation, methods for measurement and characterisation of texture and concentrates on research undertaken attempting to relate the texture of road stones to friction.
3. Feasibility studies
Relating primarily to the practical implementation aspects of this project, the experiments described in this chapter explore the feasibility of measuring texture at traffic speed and the feasibility of characterising texture using measurements made in the laboratory.
4. First attempts at an improved methodology for examination of surface texture changes
Describes an experiment using an early incarnation of the robust methodology described in the next chapter and justifies the need for careful development of such a methodology.
5. Development of a robust methodology to examine surface texture changes
Describes in detail the methodology developed, including comparisons between polishing in the laboratory and polishing by traffic, and friction testing in the laboratory and skid resistance measurement on in-service roads.
7. Quantitative analysis of changes in texture during polishing
Explains the attempts made to characterise the surface texture of aggregate surfaces and the potential for development of a numerical relationship between texture and friction.
8. Summary and discussion
Collates the findings from preceding chapters and discusses their implications.
9. Conclusions and recommendations for further work
Discusses the research presented in this thesis in the context of the research questions and the research aims posed at outset. This chapter also proposes further work that should be carried out to advance the understanding of the relationship between friction and the texture of aggregate particle surfaces.
Design Manual for Roads and Bridges. (2004, August). Volume 7 Section 3,
HD28/04, Skid resistance. London: The Stationery Office.
Department for Transport. (2011, December 15). RAS40007 Reported road
accidents and casualties: 1950 onwards. Retrieved July 20, 2012,
from DfT Tranport Statistics:
Rogers, M. P., & Gargett, T. (1991). A skidding resistance standard for the national road network. Highways And Transportation, 38, 10-16. Viner, H. E., Sinhal, R., & Parry, A. R. (2005). Linking road traffic accidents
with skid resistance - recent UK developments. International Safer
The first research aim is to develop a robust methodology for observation of aggregate particle surface texture during polishing in the laboratory. In order to tailor the methodology to allow investigation of the most pertinent features of aggregate surfaces it is necessary to develop an understanding of a range of subjects. This chapter therefore presents a review of available literature with particular attention to the topics listed below. 1. Friction theory
The mechanisms involved in opposing the movement of one body sliding against another. There are many theories about friction interaction, rigorously debated and without general consensus, and some elements are likely to be useful when considering what characteristics of a pavement surface effect and affect its skid resistance.
2. Road surface texture
Definitions of various scales of texture such as macrotexture and microtexture, the need for pavement microtexture and methods used to measure pavement texture. It has been well established that the surface texture of a pavement is a critical element of the road/tyre interaction and there exist several commonly used descriptions of surface texture. Empirical evidence has suggested that the various discrete scales of texture influence various performance criteria. The smallest scale of texture, microtexture, has the greatest influence on slow speed skid resistance in the wet, and macrotexture (the next size up) influences the speed dependence of friction seen by a sliding tyre. Macrotexture is routinely measured on pavement surfaces, but microtexture is not (although low speed skidding resistance is measured directly).
3. Texture measurement
Methods used to measure surface texture. Surface texture plays a vital role in many applications, particularly when considering machine components, and its measurement has therefore been an important exercise for many decades. Measurement of pavement surface texture is somewhat newer and there are several common techniques used in both fields.
4. Texture characterisation
Methods used to describe a surface’s texture. There are well established methods of characterising a pavement’s macrotexture, and there are standard parameters used in engineering to describe elements of a surface’s roughness. While some researchers have attempted to characterise microtexture of pavement surfaces there is no established methodology for doing so.
5. Factors (including texture) affecting skid resistance
Attempts to compare texture and skid resistance, or estimate skid resistance based on texture measurements alone. The relationship between macrotexture and the friction/speed curve has been well documented. Researchers have frequently attempted (with some success) to calculate the skid resistance expected on a surface at any speed given its skid resistance at one speed and a measure of macrotexture. However, partly because of the relative difficulty of measuring microtexture and the lack of an established method for microtexture characterisation, the link between microtexture and skid resistance is less well understood.
Characteristics of a variety of rocks used as aggregate in UK roads and standardised methods to measure their polish resistance. Different stones react to the action of polishing by traffic, and to other external factors, differently depending on their geological makeup. It will be important to consider an aggregate’s mineralogy and expected behaviour when studying its surface texture.
The research carried out for this PhD is primarily concerned with the skid resistance of the road surface (i.e. the road’s contribution to road/tyre interaction and the resultant friction force) and the characterisation of texture that affects skid resistance. To a certain extent it is independent of the added complications of tyre rubber’s behaviour and of the hydrodynamic flow of water that is frequently present on the road surface. However, in order to understand the features of road surfaces that will contribute to its skid resistance, it is necessary to first explore mechanisms of friction as a whole. Note, therefore, that this section deals primarily with theory as examined in the laboratory using idealised rubber compounds and idealised surfaces. Comments about the relevance of the theory for tyre/road interaction are made at the end of the section.
2.1.1 Classical friction
The laws of friction, as taught in schools, can be found in many texts, the first reference source in this literature review is from a well-known online encyclopaedia.
Guillaume Amontons published his laws of friction in 1699, based on notes made by Leonardo da Vinci, and they were amended by Charles-Augustin de Coulomb and Leonhard Euler. The resulting three laws of friction, which apply in dry conditions, can be summarised as (Wikipedia):
The force of friction is directly proportional to the applied load (Amontons’s 1st Law)
The force of friction is independent of the apparent area of contact (Amontons’s 2nd Law)
Kinetic friction is independent of the sliding velocity (Coulomb's Law).
Through mathematical description of the interactions, Euler also contributed a further observation:
Static friction is greater than kinetic friction. Amontons’s two laws are summarised by the equation:
where F is the force due to friction, N is the normal force and is the coefficient of friction. is specific to the two materials in contact, is dimensionless, and can only be found empirically.
Substantial further work to develop the understanding of friction was carried out by Bowden and Tabor, and they popularised the adhesion model of friction: “the frictional resistance between un-lubricated metals is due primarily to the shearing of the metallic junctions formed by adhesion and welding at the points of contact” (Bowden & Tabor, Mechanism of metallic friction, 1942). A further theory, demonstrated experimentally and published in 1950 (Bowden & Tabor, The friction and lubrication of solids, 1950), suggested that the true area of contact, being only a proportion of the apparent area of contact, even for apparently smooth surfaces, increases with increasing normal force as more asperities come into contact and those already in contact plastically deform.
David Tabor, incidentally, was part of the committee that proposed the term ‘tribology’ for the study of frictional interaction between solids (Field, 2008).
The field of study for frictional interaction between metals and other plastically deforming materials is large. Any further review of literature not dealing with rubber could be considered unproductive because rubber (and therefore any vehicle tyre) does not obey any of the above described ‘laws’ of friction. The concept of friction due to adhesion forces, and the work of Tabor, is relevant.
2.1.2 Rubber friction
Being one half of the tyre/road interaction, the properties of tyres (i.e. rubber) are very important. Rubber, both natural and synthetic, is composed of polymers (long chains of molecules linked by covalent bonding); it is a viscoelastic material. Its viscoelasticity has a direct bearing on the various theories governing frictional forces experienced when rubber is involved.
considered the force due to wear to be ‘intrinsic’ and relatively small (1-2%) in all non-emergency braking. Even in emergency braking situations, where FC is more significant, it will depend largely on the tyre
composition and is likely to be highest on those surfaces already providing high FA and FHb.
Roth, Driscoll and Holt (1942) carried out experiments to investigate the friction between rubber and hard surfaces. They used rubber specimens and testing surfaces, prepared in the laboratory, set up on a horizontal track system. The rubber specimens had a similar composition to soft rubber compounds used in vehicle tyres. Various loads were applied to the sliding rubber specimens and it was found that the coefficient of friction (Equation 2.1) decreased with increasing load. They also found that different specimen sizes exhibited different friction coefficients, so that appeared to be area dependent.
Similar experiments by Thirion (1946) led to the same conclusions: that decreases with load and is area dependent. The concept of adhesion was used to explain the friction between rubber and the smooth glass plates used.
The friction force due to adhesion is due to a molecular interaction at the sliding interface - molecular chains (polymers) in the rubber surface attempt to link with molecules in the hard surface and the bonding, stretching and breaking cycle results in a retarding force. Figure 2.1 shows a standard diagrammatic representation of the adhesion component of friction.
Figure 2.1 Friction force due to adhesion
Surf ace asperity Direction of sliding
Adhesion can be considered as a sum of forces between individual points of contact so that:
2.3 where ni is the number of molecular junctions between the surfaces at
location i and ji is the effective junction or bond strength. So, the more
points of contact, the greater the adhesive friction.
The conflict between this interpretation and Amontons’s laws was resolved for plastic deformation: the true area of contact, which, due to the presence of small asperities is smaller than the apparent area of contact, is proportional or nearly proportional to the load applied (Bowden & Tabor, 1950). This is further expanded by researchers such as Shallamach (1952) who showed that frictional force is dependent on the true area of contact and that, for rubbers, its variation with load is consistent with Hertz’s formula:
2.4 where d is the diameter of a circle formed when an elastic sphere is flattened against a hard surface, W is the normal load, r is the sphere’s radius and E is Young’s modulus of the sphere. So that the coefficient of friction becomes:
2.5 where c is a factor to be determined empirically.
Lorenz et al. (2010), who note that a full comprehension of contact between randomly rough surfaces has not yet been achieved, present two theories governing separation of two surfaces, including the difference between actual and apparent contact, when two solids are squeezed together. A simple experiment, whereby a near-elastic rubber block was pressed against an asphalt block and a concrete block in turn, showed that increasing squeezing pressure caused an exponential decrease in surface separation.
When a viscoelastic material deforms it exhibits properties of both viscous materials and elastic materials. To differentiate between viscous, elastic and viscoelastic, it is necessary to consider stress and strain. Strain, , is a measure of the relative displacement between particles in a material body in response to the application of some force, or stress, . Strain is unit-less: the length of deformation per length of original size. Stress, with units of Nm-2, is measured in relation to the unit area to which it is applied.
Viscous materials deform linearly with time under a given stress: the longer the stress is present, the greater the strain. Viscous materials do not return to their original shape when the stress is removed.
Elastic materials deform instantaneously when stress is applied and can return to their original shape when the stress is removed.
Viscoelastic materials have properties of both; the relationship between stress and strain is dependent on time and the material can return to its original shape when the stress is removed.
Tabor (1955) carried out experiments using smooth steel spheres, of various radii, rolling in rubber grooves. He found that a considerable friction force still acted even when lubricants were present separating the surfaces (so preventing, or at least suppressing, adhesion). He concluded that there must be another mechanism acting to oppose the motion of the spheres and that it must be related to the work done compressing or stretching the rubber.
When stress is applied to a purely elastic material, the material deforms instantly, and it also deforms linearly with the amount of stress applied. When the stress is removed, the material instantly returns to its original form. This can be shown in a stress-strain curve, as in Figure 2.2, which shows the stress required for any given strain (or the strain achieved at any given stress) and is the same whether loading or unloading is being performed.
Figure 2.2 Elastic stress-strain
When stress is applied to rubber, because it is viscoelastic, the deformation is not proportional to the amount of stress applied. Furthermore, as the stress is removed, the reformation of the material is neither proportional to the amount of stress, nor opposite to the amount of deformation that occurred when the stress was applied. This can be represented in a typical hysteresis loop as in Figure 2.3. As more and more stress is applied, the amount of deformation (measured by strain) increases non-linearly along the blue, loading, path (top). As stress is removed, the amount of deformation reduces more slowly at first, along the red, unloading, path (bottom).
Figure 2.3 Viscoelastic stress-strain hysteresis loop
The area under stress-strain curves is given by:
S tr e ss , Strain, S tr e ss , Strain,
multiplied by distance moved) per unit volume of material. In a hysteresis loop, the amount of energy required to deform the material (area under the blue curve) is greater than the energy released when the material reforms (area under the red curve). The difference in energy is dissipated as heat. Energy is lost as a tyre rolls over a rough surface (as in Tabor’s experiments) when the surface causes a deformation.
Because reformation is slower than deformation, when surface roughness exists, the motion of a sliding tyre causes an asymmetrical draping of rubber over a surface asperity. The rubber tends to pile up on the leading edge of the asperity and break contact with trailing edge of the asperity at a higher point. In this way, a pressure distribution is formed that has a net opposition to the direction of sliding, shown diagrammatically in Figure 2.4.
Figure 2.4 Friction force due to hysteresis
A more detailed analysis of hysteresis includes consideration that, for rubber, when a stress is applied the resulting strain can become out of phase (Roch, 1994). At low temperatures (below the ‘glass transition temperature’) polymer chains in rubber will not move about freely. At high temperatures, polymer chains are able to move and the rubber becomes almost elastic. In between these two temperatures polymer chains can move but only if there is space available to do so, which depends on the movement of other polymer chains. So, when a stress is applied it takes time for the polymer chains to align in the direction of that stress and deformation therefore lags behind the stress applied. The effect can be observed by application of a sinusoidal stress to a rubber specimen: the deformation will also be sinusoidal, but will lag behind by a phase angle. It has been shown that the hysteretic loss in the rubber is related to the tangent of this phase angle. As the frequency of the stress applied
Surf ace asperity Direction of sliding
increases, so too does the phase angle. For a sliding rubber block, the frequency of the stress applied is related to the speed of sliding and the size and spacing of surface asperities.
It is possible, apparently, to optimise the damping properties of rubber tyres so that they provide improved wet skid resistance without detrimental increase in rolling resistance (a factor not covered in this review but which is undesirable from an efficiency and environmental point of view). Rubber polymers have been developed that are tuned to generate hysteretic loss under different conditions. So, when the tyre is sliding, hysteretic loss will be greater because tyre deformations occur at higher frequencies than when the tyre is rolling (Roch, 1994).
220.127.116.11 Adhesion and hysteresis together, and further possible mechanisms
To further investigate hysteretic bulk deformation theories, Grosch (1963) carried out experiments by sliding various surfaces at different speeds against five types of rubber. While carefully controlling temperature and measuring the forces generated, he pressed flat rubber specimens against a moving track surface using a dead load suspended below. The surfaces included silicon carbide paper and smooth, but wavy, glass; the experiment was repeated for each of these surfaces after coating in a fine magnesium powder (separating rubber from the surface and suppressing adhesion). Grosch plotted master curves, using results corrected to a reference temperature, for coefficient of friction, , against the logarithm of the test surface sliding speed. He found that, on the glass surface, increased to a maximum at a particular speed, and then decreased. He noted that when the experiment was repeated on a glass surface dusted with magnesium powder, the friction measured remained almost constant over the range of speeds. For the rough silicon carbide paper surface, the -speed curve exhibited a significant peak at higher speeds, and often, a smaller peak at a lower speed, coinciding with the one found on un-dusted glass. When silicon carbide surfaces were dusted, the higher speed peak was reduced, and the lower peak was eliminated. The graph in Figure 2.5 gives a
Figure 2.5 Coefficient of friction against speed
It is thought that the adhesive interaction relies on bonds between the surface and the rubber forming and breaking. The rate at which this can occur is limited by the size of bonds and the size of polymer chains in the rubber. The maximum adhesive friction is therefore experienced at relatively low speed. Friction due to hysteretic losses depends on the frequency of application of the stress and this is related to the sliding speed and the size/spacing of asperities on the surface, which is a lot larger than the size of polymer chains. The speed at which hysteretic friction reaches a maximum is therefore generally higher. The exact speed at which these maxima occur is governed by the properties of the rubber. Savkoor (1965), Kummer (1966) and Yandell (1970), amongst others, also suggested the existence of a fourth mechanism of friction. The mechanism arises because macroscopically smooth surfaces can be microscopically rough, and micro-asperities on a rubber surface could interact with the micro-asperities on the hard surface, causing surface (as opposed to bulk-) hysteresis or ‘microhysteresis’, FHs.
In his recent book, Smith (2008) summarises the results from a number of experiments looking at the mechanisms of friction (as above) and performs back-calculations using the results. He shows that, in the majority of cases, when the total frictional force is considered in its component parts, there is a remaining unaccounted-for component. This fourth component, also attributed to ‘microhysteresis’, is independent of applied load, and is proportional to the contact area.
Sliding speed (log10
Using finite element analysis and considering either rigid spheres indenting rubber surfaces or rubber spheres sliding on rigid surfaces, Gabriel et al. (2010) suggested an additional frictional force, FGeometry, that exists in the
former but not in the latter. The magnitude of this additional mechanical force is dependent on the penetration of the rigid body into the elastomer. Further work will consider more complicated, multi-asperity surface interactions such as that of the tyre and road.
Using rubber spheres sliding on a hard surface, Schallamach (1971) observed that rather than slipping past one another, folds are generated within the contact area, known as waves of detachment (or Schallamach
waves). The waves run from the front to the rear edge of the ‘sliding’
rubber and, as with a fold in a rug that moves over a floor, the rubber can become displaced relative to the hard surface without truly sliding against it. In a more recent paper, Fukahori et al. (2010) cites a number of attempts to specifically investigate Schallamach waves. Amongst other observations it is noted that the frequency of the waves is dependent on sliding speed, Shallamach waves are not observed below a certain critical sliding velocity, and the presence of these waves reduces contact area. It should be noted, however, that the Shallamach waves are generally only observed when the elastomeric compound is very soft and the surfaces generate a very high level of friction. It has therefore been suggested that the waves are strictly an effect of friction rather than a cause of it (Savkoor A. R., 1987).
The introduction of a lubricating film between two surfaces will generally reduce the coefficient of friction, and therefore the frictional force experienced. When the two surfaces are rigid the forces experienced can be modelled using Navier-Stokes and Reynolds’s equations. Once again, rubber makes things more complicated. Except in flooded conditions, rubber will drape over asperities in a rigid surface so that there is more separation (filled with the lubricating film) in some regions than in others. Moore (1975) presents a diagrammatic representation of rubber draping,
Figure 2.6 Elastohydrodynamic separating effect in lubricated sliding
The diagram above appears to show a boundary lubrication condition, where some of the rubber is in contact with lubricant and some is in contact with the solid surface. However, during sliding, because of the flowing action of the rubber, some of the lubricant is also dragged over the asperity tips. If the asperities are smooth and rounded, complete separation may occur, drastically reducing the coefficient of friction. If there is some roughness at the asperity tips, the lubricant film is broken and adhesion can occur. This theory that road surface roughness is required to break through a lubricating film of water is revisited in Section 2.2.
If there is sufficient water on the surface (the lubricant in the case of tyre/road interaction is generally water), there are likely to be regions where the tyre does not contact the road at all. It is thought that, when a tyre rolls or slides over a wet road surface, there are three distinct zones of contact (Gough, 1974) and (Moore, 1975). The tyre squeezes water out in front of it and the front part of the tyre, in zone 1, floats on an unbroken thin film of water. Further back, in zone 2, the tyre is able to drape over the larger asperities and will begin to make actual contact with the smaller asperities. In zone 3, only a thin film of water may remain, and in this area the tyre makes contact with the surface through the film. The relative size of these three zones depends on speed, and above a critical speed there may be no contact with the pavement leading to hydroplaning.
Rubber Surface Thin lubricant film +ve -ve +ve +ve -ve -ve Elasto- hydro-dynamic pressure
Figure 2.7 Three zone contact concept from (Smith, 2008)
Considerable work has been carried out by the tyre manufacturing industry to study the mechanisms of friction between the road and their product. Indeed, a number of the papers referred to above are the result of research funded by rubber and tyre producers.
The literature has shown, as expected, that tyre/road interaction is a complex phenomenon, further complicated by the unusual and less predictable (through classical mechanics at least) behaviour of viscoelastic rubber. Smith (2008) neatly summarises results from a large number of rubber friction experiments and shows that in the vast majority, the laws of (metallic) friction do not apply.
When considering the way in which surface texture effects a road’s skid resistance, three of the well documented rubber-friction phenomena will be of particular interest:
The coefficient of friction is related to the true area of contact. The coefficient of friction is dependent on asperity distribution
It may also be useful to bear in mind that the coefficient of friction reaches a maximum as the true contact area saturates, and that there is normally a peak in friction at a given sliding speed which is dependent on material properties.
The remainder of this review will deal with the other half of the tyre/road interaction problem, (i.e. the road surface) and the next section discusses road surface texture.
Road surface texture
The previous section started with a brief review of classical friction theory. However, it was noted that the application of that theory, where the properties of rubber had not been taken into account, is not necessarily relevant to the study of tyre/road interaction. Similarly, research dealing with idealised surfaces created in the laboratory or surfaces existing only in theory, may not apply to road or aggregate surfaces.
In his thesis dealing with the dry adhesive friction of elastomers, Savkoor (1987) notes:
“...it may be argued from experience that when the many surfaces which may not be "smooth textured" initially, do become so after having "run-in" for some time so that the shapes of their asperity tips are most likely to be smooth and convex. Such smooth and convex shapes can be represented generally by a curved surface having two principal radii of curvature...” Savkoor goes on to restrict his theoretical work to the case of ideal spherical asperities.
Another frequently used simplification is that of a self-affine fractal surface (Persson, 2001). In these surfaces, given the correct scale transformation, very fine texture has the same form as texture on a larger scale, which in turn has the same form as texture on a larger scale again. Fractal dimensions will be discussed in more detail when considering methods for characterisation of surface texture.
These are common, and perhaps necessary, assumptions because rubber friction is complicated enough without also dealing with surface texture. However, since the research presented in this thesis is aimed at measurement and characterisation of surface texture (rather than a study of friction) this section skips over theoretical treatments of surface texture straight to a review of accepted definitions of road surface texture and its perceived necessity.
The geometric profile of the road in the vertical plane has traditionally been divided into different scales depending on the dynamic response of interest
1987). It should be noted that, in general, large amplitudes are desirable when wavelengths are below 10 mm and small amplitudes are desirable for wavelengths above 10 mm. The surface characteristics are divided into four general pavement surface features – unevenness, megatexture, macrotexture and microtexture – which are discussed below.
Figure 2.8 Surface texture characteristics
The unevenness of the road surface, with wavelengths from 0.5 m to 50 m, is associated with longitudinal profiles larger than the tyre footprint. It affects vehicle dynamics, ride quality, dynamic loads, and drainage. In extreme cases, unevenness can lead to loss of contact with the surface, and it is normally caused either by poor initial construction or deformation caused by loading.
The road’s megatexture refers to deviations with wavelengths from 50 mm to 500 mm. Examples of megatexture include ruts, potholes, major joints and cracks. It affects vibration in the tyre walls but not the vehicle suspension, and it is therefore strongly associated with noise and rolling resistance. Although megatexture generally has larger dimensions than those which affect skid resistance, it is possible that this scale of texture could influence tyre/road contact.
Macrotexture is the amplitude of deviations with wavelengths from 0.5 mm to 50 mm, and is effected by the size, shape, spacing and arrangement of coarse aggregate particles. Macrotexture affects
mainly tyre noise and water drainage from the tyre footprint. This scale of texture is thought to be important for hysteretic friction, especially at high speed.
Microtexture is the amplitude of deviations with wavelengths less than or equal to 0.5 mm. This scale of texture is measured on the micron scale, and is typically found on the surfaces of coarse aggregate particles (rather than being due to the gaps between them as in macrotexture) or the texture of bituminous mortar and fine material. Microtexture is frequently therefore a function of aggregate particle mineralogy and petrology and is affected by climate/weather effects and traffic action. The microtexture of the road surface is thought to affect skid resistance at all speeds for dry and wet conditions.
The scales of surface irregularities that affect skid resistance are illustrated in Table 2.1 along with terms used to describe them .
Table 2.1 Illustration of terms used to describe road surface texture
Surface Scale of texture
Macro (large) Micro (fine)
A Rough Harsh
B Rough Polished
Experimental results show that surfaces with harsh microtexture, but smooth macrotexture, have high skid resistance at low speed, but the rate at which friction reduces with increasing speed is greater than for surfaces with rough macrotexture – this is expanded in Section 2.5.
Considering a pavement under wet conditions, the presence of a thin film of water obscuring contact between the tyre and surface drives the requirement for roughness, and the shape of roughness required. The following is an analysis of the requirement for pavement roughness in wet conditions from Moore (1975).
Two extreme examples of roughness shape, the cone and the sphere, are illustrated in Figure 2.9. Let p* be the minimum pressure required to break through the water film on the surface. If a load is applied to the cone shape such that the maximum pressure exerted on the tyre, pmax, is
just more than p*, then the same load applied to the sphere will result in a maximum pressure exerted which is less than p* and no penetration of the water film can occur. However, since the cone would be subject to severe wear at its peak, a compromise between the two shapes is required.
Figure 2.9 Examples of pressure distribution in tyre surface
It is generally agreed that surface macrotexture is required in wet conditions so that the bulk of water present can be drained away and also to generate friction through tyre deformation and therefore bulk hysteresis. A surface requires microtexture so that it can break through any remaining film of water. The graph in Figure 2.10 demonstrates the trade-off between macrotexture and microtexture. On the extreme left of the graph, if the pavement has relatively smooth macrotexture, then the surface will have insufficient drainage and there will be little or no contact with the tyre regardless of the amount of microtexture present. On the extreme right of the graph, the shape of asperities and therefore the roughness of the
pmax pmean p* p re ssu re a a pmax pmean p* p re ssu re a a r
macrotexture is sufficient by itself to break through any water present on the surface; again microtexture is not necessary. Most pavement surfaces will have macrotexture somewhere in between these two extremes and microtexture, therefore, will be required for adequate friction in wet conditions.
Figure 2.10 Microtexture requirements for pavement design
Sabey (1958) investigated the friction between rubber and various sliding shapes under wet conditions. Her tests showed that the coefficient of friction under wet conditions is closely related to the pressure over the contact area between the sliders and the rubber. It was concluded that, to ensure good skid resistance in wet conditions, surface asperities should be such that average pressures of 1000 lb in-2 (approximately 6.9 MPa) are set up on them, and that individual projections should have angles at their tips of 90˚ or less. P e a k p re s s u re o n a s p e ri ty
Increasing macrotexture roughness
Increasing requirement for microtexture harshness Design range for microtexture
partly supported by asperities emerging through the water film and partly supported by the water film itself (see Section 2.1.3). Consideration of the theoretical deformation of the rubber slider alone could not differentiate between surfaces with and without microtexture and so it was concluded that an adhesion component of force, relating to the contact between the slider and the emerging asperities was required.
The texture that is generally believed to have the greatest effect on a road’s skid resistance has wavelengths lower than 50 mm and amplitudes are typically less than 5 mm (PIARC, 1987) i.e. macrotexture and microtexture. Clearly there are additional practical considerations driving the techniques that are suitable for measurement in the field, including speed, robustness and accuracy.
However, since the intention of this project is to make detailed measurements of surface texture, any device or technique that is capable of measuring texture within the specified range is potentially of relevance. This section first describes the techniques that are well established for measurement of road surface texture, then techniques that may be useful for field measurement in the future, and finally techniques that will probably only ever be possible under controlled laboratory conditions. Macrotexture is routinely measured on in-service roads and although there have been various methods employed in the past, in the UK macrotexture is now almost exclusively measured using the volumetric patch technique or using distance measuring lasers.
2.3.1 Standard methods for measuring road surface texture
The volumetric patch technique is documented in a British Standard (British Standards, 2010). A known volume of sand (or glass beads) is spread evenly over the surface to be measured, in a circular pattern. The diameter of the resulting circle of sand is measured and used to estimate the mean texture depth (MTD) of the surface. This method is accurate and repeatable and, importantly, gives a direct measurement of surface texture, but requires a stationery operator and a traffic-free road. In the UK, it is still used for new surfacing before the road is opened to traffic, and when the road is closed for other reasons (such as when cores are taken to assess structural condition). However, for large scale measurements and traffic speed surveys, distance measuring lasers are used to produce a surface profile from which texture depth can be
calculated. Servo systems are often installed in the measuring device to keep the laser at a known reference distance from the surface, allowing the small changes in distance due to surface asperities to be measured. This type of laser system is represented in Figure 2.11.
Figure 2.11 Laser triangulation
The distances measured by the laser are then used to calculate either ‘Sensor Measured Texture Depth’ (SMTD) or ‘Mean Profile Depth’ (MPD), discussed in Section 2.4, which are used as measures of macrotexture.
2.3.2 Less common or future field measurement techniques
One technique that is frequently examined for use in measurement of road surface texture is that of profile projection. Essentially, light, in a straight line, is projected onto a surface at an angle, and then photographed. The resulting image of the straight line can be used to measure surface profile directly (Forster, 1989), although the resolution of this technique depends on the image resolution and the method of measurement. The method employed by Forster is as follows: the surface is coated with white paint and a semi circle of light is projected onto the surface at an angle of 45° so that a straight line is sharply focussed on the surface. Viewed from above, the straight line traces the vertical profile of the surface which can then be photographed and measured using a microscope or by projection onto a screen with a calibrated scale.
A study to assess laser triangulation under structured lighting as a potential method for determination of road surface microtexture was carried out by Demeyere and Eugène (2004). The method described,
Target surface Reference distance Laser diode CCD
which also had applications in several areas of general metrology, used a laser to cast a line onto a road surface under test, which is observed using a digital camera. The 3D coordinates of each point on the laser curve were calculated leading to determination of the road microprofile with a claimed accuracy of approximately 10 µm.
Another commonly investigated technique is stereopsis, which is a field of photogrammetry, also referred to as stereo-photogrammetry or stereovision. Sabey and Lupton (1967) describe the technique and prototype equipment used to capture texture information about asphalt surfaces. Figure 2.12 shows a copy of the simple ray diagram they used to explain the principle. If a pencil, standing on its end, is photographed from directly above and from a position slightly displaced, the two images created when they are superimposed will also be slightly displaced. The top (T) and bottom (B) of the pencil will superpose in an image taken from directly above, at position M, when the camera lens is at position A. If the camera lens is moved a distance b to the right, to position A’, the images of the top and bottom of the pencil appear at T’ and B’ respectively. The displacement of the lens to the right is equivalent to a displacement of the pencil the same distance, b, to the left; the dashed lines show how the images of the ends of the pencil would appear at T’’ and B’’ if this were the case. When the second image is superimposed on the first, its displacement, to the right, is called its parallax.
If the parallax of the top of the pencil, the distance, MT’’, is called p then 2.7 where b is the distance between the two lens position, f is the distance between the lens and the photographic plate (or CCD sensor in a modern camera) and h is the vertical distance between the lens and the object.
Figure 2.12 Schematic for stereovision
From the ray diagram, it’s clear that this follows from observations of similar triangles. By finding the equivalent relationship for the bottom of the pencil, or by differentiation with respect to p,
2.8 where h is the height of the pencil and p is the difference in parallax, which is negative because points further away from the lens will create a displaced image closer to the original.
Millar and Woodward (2010) used a stereo vision technique to generate three-dimensional models of various road surfaces on a trip between Torino and Calais. Road surface texture measured using the models compares well with measurements made of the same surface using the volumetric patch technique. The same researchers went on to use the technique, and three-dimensional models of asphalt surfaces, to investigate tyre contact and its effect on wear and asphalt durability (2011).
A similar technique was used effectively by researchers at the SIC laboratory of the University of Poitiers and the LCPC through development of a transportable system for capturing pavement images (Slimane, Koudeir, Brochard, & Do, 2008). In this case, rather than moving the camera a known distance and taking two photographs, a camera in a fixed position was surrounded by three separate light sources. Three photographs, lit from different angles, were taken and used to calculate surface relief. A brief description of the system, and calculations, follows. The amount of light reflected by a surface element in the direction of the camera will depend on its specularity, its angle in relation to the camera
p M B'' T'' M' B' T' A' A b B T h b f h
and its colour. Colour digital images contain information about hue, saturation and intensity for each individual pixel - this is the HSI model (Wyszecki, 1982). All of this information can be used for analysis of the surface being photographed.
The assumption was made that, for surfaces of uniform colour, variations in grey-level in images were equivalent to variations in relief. This is an important assumption that will be revisited in Chapter 4. The technique using stereovision with three lighting angles was developed to improve performance on surfaces that were not uniform in colour. The images, with resolution of approximately 50 µm per pixel, were taken in turn with lighting positioned at 120° angles around the camera and focused on the image area so that the light incident on the surface was at the same angle from vertical.
It was assumed that the surface was Lambertian – light falling on the surface is diffusely reflected in such a way that the apparent brightness of the surface to an observer is the same regardless of the observer’s angle of view – and that the intensity of light reaching the camera lens is expressed by:
2.9 where (x,y) is the incidence angle of light related to the reflecting facets of the surface, r is the distance between the lighting source and the reflecting facet and L(x,y) describes the colour properties of the surface at any point.
It is then shown that the angle of incidence of light related to the reflecting facet, (x,y), can be expressed in terms of the angle of incidence of light related to the surface plane, i (for i 1, 2 or 3 for each light source), the
angle of incidence of light related to the x-axis, i (0°, 120° and 240° as
described), and the gradients of the surface facets.
Since there is one such equation, I1(x,y), I2(x,y) and I3(x,y), for each of
the three lighting angles, they can be solved to cancel the colour information L(x,y) and yield the gradients of the surface facets for each
2.3.3 Laboratory techniques for measurement of surface texture
Several of the most common techniques are described in some detail in a book on the subject of optical measurement of surface topography (Leach, 2011). It is pointless to reproduce full descriptions of all of them here. Stylus instruments are mentioned below for context and for reference when surface texture characterisation is discussed in Section 2.4. Three other techniques (laser triangulation, focus variation and scanning electron microscopy), and specific examples of the equipment using them, are discussed because they will be used in the experiments described in Chapters 3, 4 and 5.
Stylus instruments are the oldest method for measurement of surface texture: a stylus is dragged across the surface and its vertical motion is used to describe a profile along individual lines. Devices for measurement of longitudinal road profile, or for detection of rutting, such as the rolling straight edge (Young, 1977), are not entirely dissimilar, but this type of technique is unlikely to be of any practical use for measurement on scales smaller than ‘megatexture’. In particular, stylus instruments do not cope well with voids or steep slopes, and they are limited by the size of the stylus tip (too large a radius gives poor resolution, and two small a radius can damage the surface through ploughing).
The Talysurf CLI 1000, made by Taylor Hobson, can be fitted with confocal, laser triangulation and stylus gauges. In the feasibility study described in Chapter 3, a laser triangulation gauge was used, and the basic principle for this technique is described in Section 2.3.1. The gauge is positioned over the test surface and can move up and down to facilitate height measurements. The test surface, placed on a moving stage, is moved laterally, along the x-axis, to build up a series of height measurements along a profile. A three dimensional surface can be scanned by moving incrementally along the y-axis so that a number of parallel profiles can be built up. The specifications for the laser triangulation gauge define its vertical resolution as 1 µm and lateral resolution as 30 µm and a speed of measurement up to 30 mm per second (Taylor Hobson, 2004).
Focus variation, as used by the Alicona Infinite Focus (Alicona, 2011), Figure 2.13, combines the small depth of field of an optical system with vertical scanning to provide topographical information derived from the variation in focus (as the name would suggest).
Figure 2.13 Alicona Infinite Focus microscope
Using a beam splitting mirror, light emerging from a white light source is inserted into the optical path of the system and focused onto the specimen via the objective lens. Light rays reflecting from the specimen and entering the objective lens are gathered by a light sensitive sensor behind the beam splitting mirror. Due to the small depth of field of the optics, only small regions of the specimen are sharply imaged when the lens is at any given height. The lens is moved vertically along the optical axis while continuously capturing data from the surface until each region of the specimen has been imaged in sharp focus (Helmli, 2011). Figure 2.14 shows a schematic diagram of a focus variation instrument.
White light source CCD Lens Objective lens Lens Test surface Semi-transparent mirror